A DFT based study of the lowenergy electronic structures and properties of small gold clusters.


 Rafe Porter
 1 years ago
 Views:
Transcription
1 A DFT based study of the lowenergy electronic structures and properties of small gold clusters. Prashant K. Jain School of Chemistry and Biochemistry, Georgia Institute of Technology, Atlanta, GA , USA. Gold clusters Au n of size n = 2 to 12 atoms were studied by the densityfunctional theory with an abinitio pseudopotential and a generalized gradient approximation. Geometry optimizations starting from a number of initial candidate geometries were performed for each cluster size, so as to determine a number of possible lowenergy isomers for each size. Along with the lowestenergy structures, metastable structures were obtained for many cluster sizes. Interestingly, a metastable planar zigzag arrangement of Au atoms was obtained for every cluster size n 5. The stable electronic structure, binding energy, relative stability and HOMO LUMO gap for the lowestenergy isomer were calculated for each cluster size. Variation of the electronic properties with size is investigated in this paper and compared with experimental results and other calculations. Keywords: Densityfunctional theory (DFT), gold nanoclusters, abinitio. I. INTRODUCTION Gold nanoclusters are a subject of much current research due to their important role as building blocks in nanoscale electronic, 1 optical and medical diagnostic devices. 2 Besides, the optical and electronic properties of nanosized clusters are also representative of how molecular scale behavior evolves into bulk solidstate phenomena. 3 In particular, small gold clusters have attracted interest as tips and contacts in molecular electronic circuits 4 and also as potential chemical catalysts. 5 However, before such practical applications can be developed, the chemical, thermodynamic, electronic and optical properties of the nanoclusters must be established. Apart from the most stable cluster isomers, other possible lowenergy structures must also be investigated. However, direct and comprehensive experimental information of
2 smaller gold clusters is difficult to acquire. Therefore, smaller gold clusters have been theoretically investigated using abinitio computational methods over the past few years. Häkkinen and Landman 6 have investigated the lowenergy structures of gold clusters and their anions for n = 2 to 10 atoms using the densityfunctional theory (DFT) employing scalarrelativistic pseudopotentials for the 5d 10 6s 1 valence electrons of gold and a generalized gradient approximation (GGA). The same authors have also compared their DFT based electronic structure calculations of small gold cluster anions to experimental photoelectron spectroscopy (PES) data. 7 Based on similar abinitio calculations, Häkkinen et al. 8 have investigated the interaction of gaseous O 2 with small gold clusters and anions. Yang et al. 9 have investigated the lowenergy electronic structures and dielectric properties of small 2D gold clusters using the DFT method in the local density approximation (LDA). While several abinitio calculations on gold nanoclusters in the past have been limited by symmetry constraints, 10 an unconstrained global minima search 11 is necessary for exhaustive search of minima on the cluster potential energy surface, so as to be able to predict all possible lowenergy isomers. Considerable progress has been recently made towards this goal by GarzoÂn et al., 12,13 who predicted amorphous structures for the most stable isomers of intermediatesize Au n (n=38, 55,75) nanoclusters based on an exhaustive minima search using genetic optimization methods that employed classical Gupta nbody potentials. Similarly, empirical potentials have been employed in the past to determine the lowest energy structures of mediumsized gold clusters However, recently Wang and Zhao 18 have used a combined scheme of DFT with empirical genetic algorithms to generate a number of possible structural isomers for gold clusters up to 20 atoms, which were further optimized at the DFT level to determine the lowest energy structures. In contrast to these earlier calculations, the work described in this paper uses a firstprinciples method based on DFT to predict a number of possible lowenergy structural isomers for each cluster size n = 2 to 12 atoms by carrying out unconstrained geometry optimizations starting from different initial candidate geometries, similar to the methodology used by
3 Häkkinen and Landman. 6 The computational method and the calculated results are discussed in the following paper. II. COMPUTATIONAL METHOD Selfconsistentfield (SCF) electronic structure calculations were carried out on small gold clusters Au n n = 2 to 12 using the QChem package. 19 The calculations were performed with the densityfunctional theory (DFT) in the generalized gradient approximation (GGA) using the Becke3LeeYangParr (B3LYP) functional 20,21 and the StevensBaschKraussJansien Cundari (SBKJC) set 22 as the effective core potential (ECP), suitable for modeling some important relativistic effects in heavy atoms. Spinorbit corrections were not included as per this calculation scheme. The calculation scheme employed the SBKJC basis set, which is a double numerical valence basis and includes a dpolarization function. The electronic structure was obtained by solving the KohnSham equations selfconsistently. Geometry optimizations were carried out with a convergence limit of 105 a.u. on the total electronic energy. The geometry optimizations were run starting from several initial candidate geometries, ranging from an open structured arrangement of Au atoms to a closepacked structure. No symmetry constraints were imposed. Two different spin multiplicities were investigated for each cluster size: singlet/triplet for oddnumbered clusters and doublet/quartet for evennumbered clusters. The optimized electronic structure for each cluster was obtained from the Zmatrices in the Q Chem program output while electronic properties were calculated from the SCF total electronic energy and the orbital energy values. The accuracy of the chosen computational scheme was verified by a calculation of the ionization potential (IP) for the gold atom. The measured IP of the gold atom using the chosen scheme is 9.27 ev, which agrees well with the experimental value of 9.22 ev. 23 Substitution of SBKJC by the LANL2DZ ECP and basis yielded an IP value of 9.42 ev, whereas a local density approximation (LDA) resulted in an IP value of 8.78 ev. Similarly, the calculated value
4 for the IP of Au 5 as per the chosen scheme is 8.25eV, which compares well with the experimental value of 8.00eV. 24 III. RESULTS AND DISCUSSIONS A. ELECTRONIC STRUCTURES 1. OpenPacked Geometry: Metastable planar zigzag structures The initial guess geometry turned out to be an important determining factor in the calculation of the optimized electronic structure, as depicted in Fig. 1. Initial guess geometries, in the proximity of an open structured arrangement of gold atoms, result in a metastable planar zigzag arrangement of gold atoms in a chain for each cluster size n 5. However, the calculation does not predict any linear arrangement of gold atoms for n 5.The average AuAu bond distance for the planar zigzag structure is ca. 2.6 A º and the AuAuAu bond angles are ca. 126 º for all cluster sizes. Häkkinen and Landman 7 predicted a similar metastable structure for Au  4 with an exactly similar AuAu bond distance of 2.6 A º. This result is also similar to a DFT based study by SaÂnchezPortal et al., 25 which showed that gold monatomic wires exhibit a zigzag shape (with a bond distance of 2.32 A º and a bond angle of 131 º ) instead of a linear one. Only under extreme tension do the wires become linear, although this occurs just before the breaking point. Nevertheless, the ground state of the wire has a zigzag geometry with two Au atoms per unit cell. The reason for the chain taking a zigzag shape can be traced back to metallic character, which manifests itself in a tendency to increase the charge density by overlapping with neighbouring atoms so as to increase the binding energy. 26 The zigzag arrangement of atoms is thus stabilized due to the effect of symmetrybreaking, which lifts the twofold degeneracy of a particular level so also increases the coordination of each atom from two to four nearestneighbours. Zigzag arrangement of atoms has been experimentally observed in some nanowires of alkali metals 27 and is also a potential explanation of the unusually large bond distances measured in short Au nanowires
5 2. ClosePacked Geometry: Lowestenergy structures Starting from closepacked geometries for each cluster size n, a number of lowenergy metastable structures were obtained for each cluster size along with the most stable (lowestenergy) structure. The Au 2 dimer is calculated to have a bond length of 2.58 A º and an IR active vibration frequency of 176 cm 1. These values compare well with DFTLDA based calculations of Wang and Zhao (2.43 A º, 173 cm 1 ) 18 and DFTGGA calculations by Häkkinen and Landman (2.57 A º ) 6 and are close to the experimental bond length value of 2.47 A º and frequency of 191 cm For the Au 3 trimer, a D αh linear chain with a AuAu bond distance of 2.64 A º is found to be more stable than a equilateral triangle with a side of 2.69 A º, similar to a result obtained by the DFTLDA 18 which predicted a linear structure with a similar bond length of 2.67 A º as also earlier CASSCF studies. 32 Clusters containing 4 to 6 atoms have stable planar structures, as in case of other small metal clusters e.g. Na n, Ag n and Cu 33,34,35 n. In case of Au 4, the most stable structure is a D 2h rhombus, which is more stable than a square with a side of 2.69 A º and a Yshaped structure by 0.69 ev and 1.54 ev respectively. Au 5 has an almost planar trapezoidal structure with C 2v symmetry, which is more stable than a 3D trigonal bipyramidal structure by about 1.5 ev. In accordance with the results of this calculation, earlier DFTLDA 18 and DFT GGA 6 calculations have both predicted the rhombus and the trapezoidal (or Wshaped geometry ) to be the most stable geometries for Au 4 and Au 5 respectively. The most stable geometry for Au 6 is predicted to be a hexagon with a side of 2.77 A º rather than a D 3h planar triangle predicted by earlier calculations. 6,18 Photoelectron spectroscopy (PES) data show low electron affinity (EA) and large HOMOLUMO gap for Au 6, 36 which is consistent with the properties of a hexagonal structure. Au 7 has a most stable 3D pentagonal bipyramidal structure and a distorted metastable structure in agreement with Wang and Zhao. 18 Clusters of size 8 to 12 have complex irregular 3D structures. The calculated electronic structures show a transition from planar to non planar geometry at n = 7, similar to earlier DFT results, 18 though Häkkinen
6 and Landman 6 have predicted nonplanar structures from n 8. Comparing with experiment, transition to nonplanar cluster geometries has been determined to take place at n = 7 on the basis of ion mobility measurements for Au cluster cations. 37 B. ELECTRONIC PROPERTIES 1. HOMOLUMO gap The energy gap between the highest occupied orbital (HOMO) and the lowest unoccupied orbital (LUMO) for the lowest energy isomers has been calculated for each cluster size. Transition from the atomic scale to bulk metallic behavior is accompanied by a closure of the HOMOLUMO gap and development of collective electronic excitations. 38 A large HOMO LUMO gap has also been considered as an important prerequisite for the chemical stability of gold clusters. 39 Figure 2 shows the size variation of this HOMOLUMO gap (E g in ev). As seen from the plot, the HOMOLUMO energy gap shows a decreasing trend with cluster size. This is consistent with the fact that, as molecular orbitals are formed from the overlap of more and more atomic orbitals, the energy levels progressively come closer. 38 In other terms, the valence electrons are delocalized over more number of atoms as the cluster size increases. The HOMO LUMO gap values also show significant oddeven oscillations. The evennumbered clusters have a larger HOMOLUMO gap than the neighbouring oddsized ones. Oddeven alterations in the HOMOLUMO gap values have been often predicted by earlier calculations for other small metal clusters 40,41 as also small Au n clusters. 6,9,18 Most importantly, HOMOLUMO gaps evaluated from photoelectron spectroscopy (PES) data of gold cluster anions have also shown oscillations. 31,42 Oddeven oscillation behaviors can be understood by the effect of electron pairing in orbitals. Evensized clusters have an even number of s valence electrons and a doubly occupied HOMO, while it is singly occupied for oddsized clusters. The electron in a doubly occupied HOMO feels a stronger effective core potential due to the fact that the electron screening is weaker for electrons in the same orbital than for innershell electrons. It is crucial
7 to note the unusually high values of the HOMOLUMO gap at n = 2 and n = 8, unlike the HOMOLUMO gaps obtained from earlier DFT calculations 6,18. The values are however consistent with the well known fact that the HOMOLUMO gap values are particularly large for n = 2, 8, 20,, the magic numbers for electronic shell closing in small monovalent metal clusters. 43 It is possible, using other methods, to calculate the HOMOLUMO energy gap for larger gold clusters and thus study the closure of the gap and hence the onset of metallicity in gold nanostructures. 2. Binding energy and relative stability The binding energy per atom was calculated for each cluster size n as E [ ET neatom] n =, B / where E T is the total electronic energy of a cluster and E atom is the total electronic energy for gold atom. The calculated binding energies are lower than those calculated by DFTLDA. 18 However, it is known that GGA underestimates the binding energy by ev/atom with respect to LDA based values. 6,44 As a comparison, this calculation yields a value of 0.95 ev/atom for Au 2 as against a value of 1.22 ev/atom 18 by DFTLDA and an experimental value of 1.10 ev/atom. 45 Figure 3 gives the variation of the per atom binding energy E B with cluster size n. As seen in the plot, the per atom binding energy increases with cluster size. This trend is due to the increase of the average number of nearestneighbours with increasing size, thus promoting greater average number of interactions per atom. This may also be an explanation for the higher binding energy of Au 5 with respect to the planar Au 6. Towards the higher values of n, the evensized clusters show binding energies higher than their oddsized neighbours. This is due to the effect of electron pairing as explained for the oscillations in the HOMOLUMO gap. One can further calculate binding energies for clusters larger than 12 atoms using methods suitable for medium and largesized clusters and thus study how the value of the binding
8 energy evolves into the bulk cohesive energy value of 3.90 ev/ atom. 46 Further, the second difference in energy for the clusters may be calculated as, ( n) = [ E( n 1) + E( n+ 1) E( n) ] E 2, 2 where E(n) is the total energy of the cluster of size n. In cluster physics, the quantity 2 E(n) is commonly known to represent the relative stability of a cluster of size n with respect to its neighbours. 41,43,47 Also, 2 E can be directly compared to the experimental relative abundance: the peaks in 2 E are known to coincide with the discontinuities in the mass spectra. 48 Figure 4 shows a plot of 2E as a function of the cluster size n. As seen, the plot shows oddeven alterations, similar to oscillations in the HOMOLUMO gap, thus predicting a higher relative stability for evensized clusters. However, a higher stability is predicted for n = 5 than n = 6, which may be due to the higher number of nearest neighbours per atom for Au 5 than for the planar Au 6. Also, magicsized clusters n = 2, 8 so also n = 10 show a higher stability. IV. SUMMARY Thus the lowenergy geometries, binding energy, relative stability and HOMOLUMO gap of gold clusters Au n, n varying from 2 to 12 atoms were investigated using a DFT based method. Table 1 summarizes the structure and properties of the lowestenergy isomer for each cluster size n. It was found that different initial guess geometries lead to a number of structural isomers for each cluster size. Most interestingly, for cluster sizes n 5, open structured guess geometries predict an additional metastable planar zigzag arrangement of gold atoms. The calculated lowest energy structures show that the smallest gold clusters are planar and a transition to a 3D structure takes place at a size of 7 atoms. Oddeven alterations are evident in the HOMOLUMO gaps and second energy differences. Evennumbered clusters show relatively higher stability. The calculated results are found to compare well with experimental data and earlier theoretical investigations of gold nanoclusters so also are consistent with
9 theoretical concepts of magic numbers and shell models. However, due to the required computational effort, this firstprinciples method is appropriate only for small gold clusters. 49,50 Medium and largesized clusters should be appropriately studied using methods employing empirical potentials, to be able to accomplish a more thorough study of the size evolution of properties in gold nanostructures. ACKNOWLEDGEMENTS I would like to thank Prof. C.David Sherill for his advice so also for providing the computational facilities at the CCMST, Georgia Tech for this work.
10 REFERENCES 1. A. C. Templeton, W. P. Wuelfing, R. W. Murray, Acc.Chem. Res. 33, 27 (2000). 2. R. Elghanian, J. J. Storhoff, R. C. Mucic, R. L. Letsinger, C. A. Mirkin, Science 277, 1078 (1997). 3. S. Chen, R. S. Ingram, M. J. Hostetler, J.J. Pietron, R. W. Murray, T. Schaaff, J.T. Khoury, M. Alvarez, R. L. Whetten, Science 280, 2098 (1998). 4. F.R. F. Fan, A. J. Bard, Science 277, 1791 (1997). 5. M. Valden, X. Lai, D. W. Goodman, Science 281, 1647 (1998). 6. H. Häkkinen, U. Landman, Phys. Rev. B (Rapid Comm.) 62, R2287 (2000). 7. H. Häkkinen, B.Yoon, U. Landman, X.Li, H.J. Zhai, L.S. Wang, J. Phys. Chem.A 107, 6168 (2003). 8. B. Yoon, H. Häkkinen, U. Landman, J. Phys. Chem.A 107, 4066 (2003). 9. Jin Zhao, Jinlong Yang, J. G. Hou, Phys.Rev.B 67, (2003). 10. C.L. Cleveland, U. Landman, T.G. Schaaff, M.N. Shafigullin, P.W. Stephens, R.L. Whetten, Phys. Rev. Lett. 79, 1873 (1997). 11. I. L. GarzoÄn, A. PosadaAmarillas, Phys. Rev. B 54, (1996). 12 I. L. GarzoÄn, K. Michaelian, M. R. BeltraÂn, A. PosadaAmarillas, P. OrdejoÂn, E. Artacho, D. SaÂnchezPortal, J. M. Soler, Phys. Rev. Lett. 81, 1600 (1998). 13. J. M. Soler, M. BeltraÂn, K.Michaelian, I. L. GarzoÄn, P. OrdejoÂn, D. SaÂnchezPortal, E. Artacho, Phys. Rev. B 61, 5771, (2000). 14. K. Michaelian, N. Rendon, I.L. GarzoÄn, Phys. Rev. B 60, 1999 (2000). 15. N.T. Wilson, R.L. Johnston, Eur. Phys. J. D 12, 161 (2000). 16. J.M. Soler, I.L. GarzoÄn, J.D. Joannopoulos, Solid State Commun. 117, 621, (2001). 17. I.L. GarzoÄn, M.R. Beltrán, G. González, I. GutíerrezGonzález, K. Michaelian, J.A. ReyesNava, J.I. RodríguezHernández, Eur. Phys. J. D 24, 105 (2003). 18. J. Wang, G. Wang, J. Zhao, Phys.Rev.B 66, , (2002). 19. C.A. White, QCHEM, Version 1.2., QChem, Inc., Pittsburgh, PA, A. D. Becke, J. Chem. Phys. 98, 5648 (1993). 21. C. Lee, W. Yang, R. G. Parr, Phys. Rev. B 37, 785 (1988).
11 22. J. J. Belbruno, Heteroatom Chemistry 9, 651 (1998). 23. C. Kittle, Introduction to Solid State Physics, 7th ed.wiley, New York, C. Jackschath, I. Rabin, W. Schulze, B. Bunsenges, Phys.Chem. 86, 1200 (1992). 25. D. SaÂnchezPortal, J. Junquera, P. OrdejoÂn, A. GarcõÂa, E. Artacho, J. M. Soler, Phys. Rev.Lett. 83, 3884 (1999). 26. C. A. Stafford, D. Baeriswyl, J. Bürki, Phys. Rev. Lett. 79, 2863 (1997). 27. L. J. Whitman, J. A. Stroscio, R. A. Dragoset, R. J. Celotta, Phys. Rev. Lett. 66,1338 (1991). 28. H. Ohnishi, Y. Kondo, K. Takayanagi, Nature 395, 780 (1998). 29. A. I. Yanson, G. Rubio Bollinger, H. E. van den Brom, N. AgraõÈt, J. M. van Ruitenbeek, Nature 395, 783 (1998). 30. Y. Kondo, K. Takayanagi, Bull. Am. Phys. Soc. 44, 312 (1999). 31. J.Ho, K. M. Ervin, W. C. Lineberger, J. Chem. Phys. 93, 6987 (1990). 32. K.G. Balasubramanian, M.Z. Liao, J. Chem. Phys. 86, 5587 (1987). 33. U. Röthlisberger, W. Andreoni, J. Chem. Phys. 94, 8129 (1991). 34. V. BonačićKouteckŷ, L. Cespiva, P. Fantucci, J. Kouteckŷ, J.Chem. Phys. 98, 7981 (1993). 35. C. Massobrio, A. Pasquarello, A. Dal Corso, J. Chem. Phys. 109, 6626 (1998). 36. K.J. Taylor, C. Jin, J. Conceicao, O. Cheshnovsky, B.R. Johnson, P.J. Nordlander, R.E. Smalley, J. Chem. Phys. 93, 7515 (1991). 37. S. Gilb, P. Weis, F. Furche, R. Ahlrichs, M. M. Kappes, J. Chem. Phys. 116, 4094 (2002). 38. N. Nilius, T. M. Wallis, W. Ho, Science 297, 1853 (2002). 39. J. Li, X. Li, H.J. Zhai, L.S. Wang, Science 299, 864 (2003). 40. J.Wang, G. Wang, J. Zhou, Phys. Rev. B. 64, (2003). 41. J. Zhao, Eur. Phys. J. D 14, 309 (2000). 42. K.J. Taylor, C.L. PettietteHall, O. Cheshnovsky, R.E. Smalley, J. Chem. Phys. 96, 3319 (1992). 43. W. A. de Heer, Rev. Mod. Phys. 65, 611 (1993). 44. O. D. Häberlen, S.C. Chung, M. Stener, N. Rösch, J.Chem.Phys. 106, 5189 (1997).
12 45. American Institute of Physics Handbook,McGrawHill, NewYork, CRC Handbook of Chemistry and Physics, edited by R. C. Weast, 64 ed.crc Press, Boca Raton; FL, C.Yannouleas U.Landman, Phys. Rev.B 54, 7690 (1996). 48. K. Clemenger, Phys. Rev. B 32,1359 (1985). 49. V. BonačićKouteckŷ, P. Fantucci, J. Kouteckŷ, Chem. Rev. 91, 1035 (1991). 50. N. Barnett, U. Landman, G. Rajagopal, Phys. Rev. Lett. 67, 3058 (1991).
13 Initia l candidate geo metry Lowenergy geometry Open structured Optimization Close packed Fig.1. Initial candidate geometry determines the optimized lowenergy geometry, for instance for n = Eg(eV) n Fig.2. Plot of HOMOLUMO gaps for different cluster sizes
14 EB(eV/atom) n Fig.3. Binding energy/atom vs. cluster size n E(eV) n Fig.4. Second energy difference in total energy as a function of cluster size
15 E g E B n Stable geometry (ev) (ev/atom) 2 dimer linear chain rhombus trapezoidal hexagonal pentagonal bipyramidal irregular irregular irregular irregular irregular Table 1.Stable geometry, HOMOLUMO gap & binding energy/atom for Au n, n = 212
Structural and Electronic Properties of Small Silicon Nanoclusters
Structural and Electronic Properties of Small Silicon Nanoclusters Prabodh Sahai Saxena a* and Amerendra Singh Sanger b a Physics Department, Lakshmi Narain College of Technology Excellence, Bhopal, India.
More informationG. Gantefdr and W. Eberhardt Institut fiir Festkiirperforschung, Forschungszentrum Jiilich, 5170 Jiilich, Germany
Shell structure and sp hybridization in small aluminum clusters G. Gantefdr and W. Eberhardt Institut fiir Festkiirperforschung, Forschungszentrum Jiilich, 5170 Jiilich, Germany Photoelectron spectra
More informationarxiv:condmat/ v1 [condmat.mtrlsci] 26 Aug 2003
Circular dichroism simulated spectra of chiral gold nanoclusters: A dipole approximation arxiv:condmat/0308552v1 [condmat.mtrlsci] 26 Aug 2003 Carlos E. RománVelázquez, 1 Cecilia Noguez, 2, and Ignacio
More informationFragmentation Behavior and Ionization Potentials of Lead Clusters Pb n (n 30)
CHEM. RES. CHINESE UNIVERSITIES 2010, 26(6), 996 1001 Fragmentation Behavior and Ionization Potentials of Lead Clusters Pb n (n 30) LI Xiaoping 1, ZHANG Wei 1, LÜ Wencai 1,2*, WANG Caizhuang 3 and HO
More informationDensity Functional Theory Calculation of the Electronic Structure for C 20 Cage Fullerene حسابات نظرية دالة الكثافة للتركيب االلكتروني للفوليرين C 20
Density Functional Theory Calculation of the Electronic Structure for C 20 Cage Fullerene حسابات نظرية دالة الكثافة للتركيب االلكتروني للفوليرين C 20 محمد اف ارح هادي هاشم نضال هادي طالب ليث عبيس اب ارهيم
More informationPeriodic Trends in Properties of Homonuclear
Chapter 8 Periodic Trends in Properties of Homonuclear Diatomic Molecules Up to now, we have discussed various physical properties of nanostructures, namely, twodimensional  graphenelike structures:
More informationIn search of a structural model for a thiolateprotected Au 38. cluster
In search of a structural model for a thiolateprotected Au 38 cluster Deen Jiang, *, Weidong Luo,, Murilo L. Tiago, and Sheng Dai Chemical Sciences Division and Materials Science and Technology Division,
More informationCHAPTER 4 Structure, Optical and Reactivity Analysis of Platinum Cluster 4.1 Introduction
CHAPTER 4 Structure, Optical and Reactivity Analysis of Platinum Cluster 4.1 Introduction Platinum clusters and other transition metal clusters like, Rh, and Pd are used as catalysts for reducing toxic
More informationDFT EXERCISES. FELIPE CERVANTES SODI January 2006
DFT EXERCISES FELIPE CERVANTES SODI January 2006 http://www.csanyi.net/wiki/space/dftexercises Dr. Gábor Csányi 1 Hydrogen atom Place a single H atom in the middle of a largish unit cell (start with a
More informationThe Boron Buckyball has an Unexpected T h Symmetry
The Boron Buckyball has an Unexpected T h Symmetry G. Gopakumar, Minh Tho Nguyen, and Arnout Ceulemans* Department of Chemistry and Institute for Nanoscale Physics and Chemistry, University of Leuven,
More informationChemical Bonding Forces and Metallization of Hydrogen
Chemical Bonding Forces and Metallization of Hydrogen Ivan I. Naumov Geophysical Laboratory, Carnegie Institution of Washington Naumov & Hemley, Accts. Chem. Res., 47(12), 3551 (2014) Importance of Fundamental
More informationElectronegativity is a very useful concept for the explanation or understanding of chemical reactivity throughout the periodic table.
1.6. Review of Electronegativity (χ) CONCEPT: Electronegativity is a very useful concept for the explanation or understanding of chemical reactivity throughout the periodic table. There are many definitions
More informationBoron Fullerenes: A FirstPrinciples Study
Nanoscale Res Lett (2008) 3:49 54 DOI 10.1007/s1167100791131 NANO EXPRESS Boron Fullerenes: A FirstPrinciples Study Nevill Gonzalez Szwacki Received: 11 November 2007 / Accepted: 4 December 2007 /
More informationExplaining the apparent arbitrariness of the LDA1/2 selfenergy. correction method applied to purely covalent systems
Explaining the apparent arbitrariness of the LDA1/2 selfenergy correction method applied to purely covalent systems KanHao Xue, 1,2 Leonardo R. C. Fonseca, 3 and XiangShui Miao 1,2 1 School of Optical
More informationReduction of Nitrogen Oxides (NO x ) by Superalkalis
Reduction of Nitrogen Oxides (NO x ) by Superalkalis Ambrish Kumar Srivastava P. G. Department of Physics, Veer Kunwar Singh University, Ara802301, Bihar, India Email: ambrishphysics@gmail.com 1 Abstract
More informationNovel structures and energy spectra of hydroxylated SiO 2 8 based clusters: Searching for the magic SiO 2 8 O 2 H 3 cluster
THE JOURNAL OF CHEMICAL PHYSICS 122, 114303 2005 Novel structures and energy spectra of hydroxylated SiO 2 8 based clusters: Searching for the magic SiO 2 8 O 2 H 3 cluster S. T. Bromley a Department
More informationDelocalized electronic states in small clusters. Comparison of Na,, Cu,, Ag,, and Au, clusters
Delocalized electronic states in small clusters. Comparison of Na,, Cu,, Ag,, and Au, clusters H. Handschuh a, ChiaYen Cha, H. Mijller b, P.S. Bechthold a, G. Gantefdr, W. Eberhardt a * Institut fiir
More informationElectronic Supplementary Information
Electronic Supplementary Material (ESI) for Physical Chemistry Chemical Physics. This journal is the Owner Societies 2014 Electronic Supplementary Information Rational modifications on champion porphyrin
More informationCalculation of Ionization Energy and Electron Affinity of Molecule of Hydro and Fluorinefullerenes C 60 H(F) n (0 n 60)
1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22 23 24 25 26 27 28 29 30 31 32 33 34 35 36 37 38 39 40 41 42 FULLERENES, NANOTUBES, AND CARBON NANOSTRUCTURES Vol. 12, No. 1, pp. 513 519, 2004 Calculation
More informationStructure, Electronic and Nonlinear Optical Properties of Furyloxazoles and Thienyloxazoles
Journal of Physics: Conference Series PAPER OPEN ACCESS Structure, Electronic and Nonlinear Optical Properties of Furyls and Thienyls To cite this article: Ozlem Dagli et al 6 J. Phys.: Conf. Ser. 77 View
More informationRDCH 702 Lecture 4: Orbitals and energetics
RDCH 702 Lecture 4: Orbitals and energetics Molecular symmetry Bonding and structure Molecular orbital theory Crystal field theory Ligand field theory Provide fundamental understanding of chemistry dictating
More informationChapter 7. Generally, the electronic structure of atoms correlates w. the prop. of the elements
Chapter 7 Periodic Properties of the Elements I) Development of the P.T. Generally, the electronic structure of atoms correlates w. the prop. of the elements  reflected by the arrangement of the elements
More information17/11/2010. Lewis structures
Reading assignment: 8.58.8 As you read ask yourself: How can I use Lewis structures to account for bonding in covalent molecules? What are the differences between single, double and triple bonds in terms
More informationInfluence of Sodium Loading on CO Adsorption over Faujasite Zeolite Supported Gold Monomers: a Density Functional Study
Review of Applied Physics Vol. 2 Iss. 2, June 2013 www.seipub.org/rap Influence of Sodium Loading on CO Adsorption over Faujasite Zeolite Supported Gold Monomers: a Density Functional Study Ajanta Deka
More informationarxiv:condmat/ v1 [condmat.meshall] 6 Sep 2002
Nonlinear currentinduced forces in Si atomic wires arxiv:condmat/963v [condmat.meshall] 6 Sep Zhongqin Yang and Massimiliano Di Ventra[*] Department of Physics, Virginia Polytechnic Institute and State
More informationCHAPTER 6 CHEMICAL BONDING SHORT QUESTION WITH ANSWERS Q.1 Dipole moments of chlorobenzene is 1.70 D and of chlorobenzene is 2.5 D while that of paradichlorbenzene is zero; why? Benzene has zero dipole
More informationMolecular Orbital Theory. Molecular Orbital Theory: Electrons are located in the molecule, not held in discrete regions between two bonded atoms
Molecular Orbital Theory Valence Bond Theory: Electrons are located in discrete pairs between specific atoms Molecular Orbital Theory: Electrons are located in the molecule, not held in discrete regions
More informationAb initio study of CNT NO 2 gas sensor
Chemical Physics Letters 387 (2004) 271 276 www.elsevier.com/locate/cplett Ab initio study of CNT NO 2 gas sensor Shu Peng a, *, Kyeongjae Cho a, Pengfei Qi b, Hongjie Dai b a Department of Mechanical
More informationProperties of Individual Nanoparticles
TIGP Introduction technology (I) October 15, 2007 Properties of Individual Nanoparticles Clusters 1. Very small  difficult to image individual nanoparticles. 2. New physical and/or chemical properties
More informationComputational Methods. Chem 561
Computational Methods Chem 561 Lecture Outline 1. Ab initio methods a) HF SCF b) PostHF methods 2. Density Functional Theory 3. Semiempirical methods 4. Molecular Mechanics Computational Chemistry " Computational
More informationSupplemental Material: Experimental and Theoretical Investigations of the Electronic Band Structure of MetalOrganic Framework of HKUST1 Type
Supplemental Material: Experimental and Theoretical Investigations of the Electronic Band Structure of MetalOrganic Framework of HKUST1 Type Zhigang Gu, a Lars Heinke, a,* Christof Wöll a, Tobias Neumann,
More informationElectron Affinities of Selected Hydrogenated Silicon Clusters (Si x H y, x ) 17, y ) 015) from Density Functional Theory Calculations
J. Phys. Chem. A 2000, 104, 60836087 6083 Electron Affinities of Selected Hydrogenated Silicon Clusters (Si x H y, x ) 17, y ) 015) from Density Functional Theory Calculations Mark T. Swihart Department
More informationAdsorption of Atomic H and O on the (111) Surface of Pt 3 Ni Alloys
J. Phys. Chem. B 2004, 108, 83118323 8311 Adsorption of Atomic H and O on the (111) Surface of Pt 3 Ni Alloys Timo Jacob and William A. Goddard, III* Materials and Process Simulation Center, Beckman Institute
More informationPractical Advice for Quantum Chemistry Computations. C. David Sherrill School of Chemistry and Biochemistry Georgia Institute of Technology
Practical Advice for Quantum Chemistry Computations C. David Sherrill School of Chemistry and Biochemistry Georgia Institute of Technology Choice of Basis Set STO3G is too small 631G* or 631G** 6 probably
More informationA study of nickel monoxide (NiO), nickel dioxide (ONiO), and Ni(O 2 ) complex by anion photoelectron spectroscopy
A study of nickel monoxide (NiO), nickel dioxide (ONiO), and Ni(O 2 ) complex by anion photoelectron spectroscopy Hongbin Wu and LaiSheng Wang Department of Physics, Washington State University, Richland,
More informationAb initio study of helical silver singlewall nanotubes and nanowires. S.L. Elizondo and J.W. Mintmire
Ab initio study of helical silver singlewall nanotubes and nanowires S.L. Elizondo and J.W. Mintmire Oklahoma State University, Dept. of Physics, Stillwater, OK 74078 Received Date: We report results for
More informationNew Magic Numbers in Ti x C y Anion Clusters and Implications for the Growth Mechanisms of Titanium Carbide Clusters
6556 J. Am. Chem. Soc. 1998, 120, 65566562 New Magic Numbers in Ti x C y Anion Clusters and Implications for the Growth Mechanisms of Titanium Carbide Clusters LaiSheng Wang,*,, XueBin Wang, Hongbin
More informationAtomic orbitals of finite range as basis sets. Javier Junquera
Atomic orbitals of finite range as basis sets Javier Junquera Most important reference followed in this lecture in previous chapters: the many body problem reduced to a problem of independent particles
More informationTeoría del Funcional de la Densidad (Density Functional Theory)
Teoría del Funcional de la Densidad (Density Functional Theory) Motivation: limitations of the standard approach based on the wave function. The electronic density n(r) as the key variable: Functionals
More informationBinding energy of bilayer graphene and Electronic properties of oligoynes
Binding energy of bilayer graphene and Electronic properties of oligoynes E. Mostaani and N. Drummond Thursday, 31 July 2014 Van der Waals interaction Important contributions to the description of binding
More informationMomentum filtering effect in molecular wires
PHYSICAL REVIEW B 70, 195309 (2004) Momentum filtering effect in molecular wires ChaoCheng Kaun, 1, * Hong Guo, 1 Peter Grütter, 1 and R. Bruce Lennox 1,2 1 Center for the Physics of Materials and Department
More informationSurface Transfer Doping of Diamond by Organic Molecules
Surface Transfer Doping of Diamond by Organic Molecules Qi Dongchen Department of Physics National University of Singapore Supervisor: Prof. Andrew T. S. Wee Dr. Gao Xingyu Scope of presentation Overview
More informationStrong Correlation Effects in Fullerene Molecules and Solids
Strong Correlation Effects in Fullerene Molecules and Solids Fei Lin Physics Department, Virginia Tech, Blacksburg, VA 2461 Fei Lin (Virginia Tech) Correlations in Fullerene SESAPS 211, Roanoke, VA 1 /
More informationAqeel Mohsin Ali. Molecular Physics Group, Department of Physics, College of Science, University of Basrah, Basrah, Iraq
Journal of Physical Science, Vol. 23(2), 85 90, 2012 Theoretical Investigation for Neon Doping Effect on the Electronic Structure and Optical Properties of Rutile TiO 2 for Photocatalytic Applications
More informationwith the larger dimerization energy also exhibits the larger structural changes.
A7. Looking at the image and table provided below, it is apparent that the monomer and dimer are structurally almost identical. Although angular and dihedral data were not included, these data are also
More informationAtoms and Periodic Properties
Chemistry, The Central Science, 10th edition Theodore L. Brown; H. Eugene LeMay, Jr.; and Bruce E. Bursten Unit 01 (Chp 6,7): Atoms and Periodic Properties John D. Bookstaver St. Charles Community College
More informationPeriodic Relationships
Periodic Relationships 1 Tabulation of Elements Mendeleev (1869) Arranged by mass Tabulation by chem.& physical properties Predicted missing elements and properties 2 Modern Periodic Table Argon vs. potassium
More informationValence Bond Theory Considers the interaction of separate atoms brought together as they form a molecule. Lewis structures Resonance considerations
CHEM 511 chapter 2 page 1 of 11 Chapter 2 Molecular Structure and Bonding Read the section on Lewis dot structures, we will not cover this in class. If you have problems, seek out a general chemistry text.
More informationGeneralized generalized gradient approximation: An improved densityfunctional theory for accurate orbital eigenvalues
PHYSICAL REVIEW B VOLUME 55, NUMBER 24 15 JUNE 1997II Generalized generalized gradient approximation: An improved densityfunctional theory for accurate orbital eigenvalues Xinlei Hua, Xiaojie Chen, and
More informationCalculating Band Structure
Calculating Band Structure Nearly free electron Assume plane wave solution for electrons Weak potential V(x) Brillouin zone edge Tight binding method Electrons in local atomic states (bound states) Interatomic
More informationPBS: FROM SOLIDS TO CLUSTERS
PBS: FROM SOLIDS TO CLUSTERS E. HOFFMANN AND P. ENTEL Theoretische Tieftemperaturphysik GerhardMercatorUniversität Duisburg, Lotharstraße 1 47048 Duisburg, Germany Semiconducting nanocrystallites like
More informationSupplementary Note 1: Dark field measurements and Scattering properties of NPoM geometries
Supplementary Note 1: Dark field measurements and Scattering properties of NPoM geometries Supplementary Figure 1: Dark field scattering properties of individual nanoparticle on mirror geometries separated
More informationValence bond theory accounts, at least qualitatively, for the stability of the covalent bond in terms of overlapping atomic orbitals.
Molecular Orbital Theory Valence bond theory accounts, at least qualitatively, for the stability of the covalent bond in terms of overlapping atomic orbitals. Using the concept of hybridization, valence
More informationCHEM 344 Molecular Modeling
CHEM 344 Molecular Modeling The Use of Computational Chemistry to Support Experimental Organic Chemistry Part 1: Molecular Orbital Theory, Hybridization, & Formal Charge * all calculation data obtained
More informationOutline. Introduction: graphene. Adsorption on graphene:  Chemisorption  Physisorption. Summary
Outline Introduction: graphene Adsorption on graphene:  Chemisorption  Physisorption Summary 1 Electronic band structure: Electronic properties K Γ M v F = 10 6 ms 1 = c/300 massless Dirac particles!
More informationEffects of Confinement on Structural Stability and Electronic Structure of Sodium Clusters
Effects of Confinement on Structural Stability and Electronic Structure of Sodium Clusters Balasaheb J. Nagare 1, Sunil P. Chavan 2 1,2Department of Physics, University of Mumbai, Santacruz (E), Mumbai
More informationAdditional information on J. Chem. Phys. Florian Göltl and Jürgen Hafner
Structure and properties of metalexchanged zeolites studied using gradientcorrected and hybrid functionals. II. Electronic structure and photoluminescence spectra Florian Göltl and Jürgen Hafner Citation:
More informationElectronic Structure Models
Electronic Structure Models Hückel Model (1933) Basic Assumptions: (a) One orbital per atom contributes to the basis set; all orbitals "equal" (b) The relevant integrals involving the Hamiltonian are α
More informationTOPIC 4 ANSWERS & MARK SCHEMES QUESTIONSHEET 1 IONIC BONDING
TOPIC 4 ANSWERS & MARK SCEMES QUESTIONSEET 1 IONIC BONDING a) A bond formed by the complete transfer of one or more electrons from one atom to another to form ions of opposite charge which attract each
More informationDEVELOPMENT OF THE PERIODIC TABLE
DEVELOPMENT OF THE PERIODIC TABLE Prior to the 1700s, relatively few element were known, and consisted mostly of metals used for coinage, jewelry and weapons. From early 1700s to mid1800s, chemists discovered
More informationThe many forms of carbon
The many forms of carbon Carbon is not only the basis of life, it also provides an enormous variety of structures for nanotechnology. This versatility is connected to the ability of carbon to form two
More informationBe H. Delocalized Bonding. Localized Bonding. σ 2. σ 1. Two (sp1s) BeH σ bonds. The two σ bonding MO s in BeH 2. MO diagram for BeH 2
The Delocalized Approach to Bonding: The localized models for bonding we have examined (Lewis and VBT) assume that all electrons are restricted to specific bonds between atoms or in lone pairs. In contrast,
More informationBe H. Delocalized Bonding. Localized Bonding. σ 2. σ 1. Two (sp1s) BeH σ bonds. The two σ bonding MO s in BeH 2. MO diagram for BeH 2
The Delocalized Approach to Bonding: The localized models for bonding we have examined (Lewis and VBT) assume that all electrons are restricted to specific bonds between atoms or in lone pairs. In contrast,
More informationneed another quantum number, m s it is found that atoms, substances with unpaired electrons have a magnetic moment, 2 s(s+1) where {s = m s }
M polyelectronic atoms need another quantum number, m s it is found that atoms, substances with unpaired electrons have a magnetic moment, 2 s(s+1) where {s = m s } Pauli Exclusion Principle no two electrons
More informationElectronic structure and bonding in metal phthalocyanines, Metal=Fe, Co, Ni, Cu, Zn, Mg
Utah State University DigitalCommons@USU Chemistry and Biochemistry Faculty Publications Chemistry and Biochemistry 2001 Electronic structure and bonding in metal phthalocyanines, Metal=Fe, Co, Ni, Cu,
More informationDesign of nanomechanical sensors based on carbon nanoribbons and nanotubes in a distributed computing system
Design of nanomechanical sensors based on carbon nanoribbons and nanotubes in a distributed computing system T. L. Mitran a, C. M. Visan, G. A. Nemnes, I. T. Vasile, M. A. Dulea Computational Physics and
More informationChapter 10 Theories of Covalent Bonding
Chapter 10 Theories of Covalent Bonding 1 Atomic Orbitals Molecules Bonding and 2 Molecular Structure Questions How are molecules held together? Why is O 2 paramagnetic? And how is this property connected
More informationJournal of Physical and Theoretical Chemistry
Journal of Physical and Theoretical Chemistry of Islamic Azad University of Iran, 9 (4) 255262: Winter 2013 (J. Phys. Theor. Chem. IAU Iran) ISSN 17352126 Theoretical thermodynamic study of CO and O
More informationCHAPTER 8. EXPLORING THE EFFECTS OF STRUCTURAL INSTABILITIES AND OF TRIPLET INSTABILITY ON THE MI PHASE TRANSITION IN (EDOTTF)2PF6.
CHAPTER 8. EXPLORING THE EFFECTS OF STRUCTURAL INSTABILITIES AND OF TRIPLET INSTABILITY ON THE MI PHASE TRANSITION IN (EDOTTF)2PF6. The thermal metalinsulator phase transition in (EDOTTF)2PF6 is attributed
More informationCalculation and Analysis of the Dielectric Functions for BaTiO 3, PbTiO 3, and PbZrO 3
CHINESE JOURNAL OF PHYSICS VOL. 1, NO. 3 June 213 Calculation and Analysis of the Dielectric Functions for BaTiO 3, PbTiO 3, and PbZrO 3 Chao Zhang and Dashu Yu School of Physics & Electronic Information
More informationDFT calculations of NMR indirect spin spin coupling constants
DFT calculations of NMR indirect spin spin coupling constants Dalton program system Program capabilities Density functional theory Kohn Sham theory LDA, GGA and hybrid theories Indirect NMR spin spin coupling
More informationATOMIC STRUCTURE, ELECTRONS, AND PERIODICITY
ATOMIC STRUCTURE, ELECTRONS, AND PERIODICITY All matter is made of atoms. There are a limited number of types of atoms; these are the elements. (EU 1.A) Development of Atomic Theory Atoms are so small
More informationThe Nature of the Interlayer Interaction in Bulk. and FewLayer Phosphorus
Supporting Information for: The Nature of the Interlayer Interaction in Bulk and FewLayer Phosphorus L. Shulenburger, A.D. Baczewski, Z. Zhu, J. Guan, and D. Tománek, Sandia National Laboratories, Albuquerque,
More informationCarbon string structures: Firstprinciples calculations of quantum conductance
Carbon string structures: Firstprinciples calculations of quantum conductance R. T. Senger, S. Tongay, S. Dag, E. Durgun, and S. Ciraci* Department of Physics, Bilkent University, 06800 Ankara, Turkey
More informationFirstPrinciple Studies on Adsorption of Cu + and Hydrated Cu + Cations on Clean Si(111) Surface
CHEM. RES. CHINESE UNIVERSITIES 2010, 26(3), 472 478 FirstPrinciple Studies on Adsorption of Cu + and Hydrated Cu + Cations on Clean Si(111) Surface CHENG Fengming 1,2, SHENG Yongli 1,3, LI Menghua
More informationNotes. Rza Abbasoglu*, Abdurrahman Atalay & Ahmet Şenocak. Indian Journal of Chemistry Vol. 53A, March, 2014, pp
Indian Journal of Chemistry Vol. 53A, March, 2014, pp. 288293 Notes DFT investigations of the DielsAlder reaction of fulvene with tetracyclo[6.2.2.1 3,6.0 2,7 ]trideca4,9,11triene 9,10dicarboxylic
More informationAsymmetry of Endofullerenes with Silver Atoms
Asymmetry of Endofullerenes with Silver Atoms V.S. Gurin PhysicoChemical Research Institute, Belarusian State University Leningradskaja str., 14, Minsk, 220080, BELARUS; Email: gurin@bsu.by; gurinvs@lycos.com
More information4 Diatomic molecules
s manual for Burrows et.al. Chemistry 3 Third edition 4 Diatomic molecules Answers to worked examples WE 4.1 The Lewis model (on p. 174 in Chemistry 3 ) Use the Lewis model to describe the bonding in (a)
More informationGeometry and electronic structure of Vn(Bz)(m) complexes
Virginia Commonwealth University VCU Scholars Compass Physics Publications Dept. of Physics 2004 Geometry and electronic structure of Vn(Bz)(m) complexes Anil K. Kandalam Virginia Commonwealth University
More informationFlatbands in 2D boroxinelinked covalent organic frameworks
Electronic Supplementary Material (ESI) for Physical Chemistry Chemical Physics. This journal is the Owner Societies 215 Supplementary Material Flatbands in 2D boroxinelinked covalent organic frameworks
More informationNo Brain Too Small CHEMISTRY AS91390 Demonstrate understanding of thermochemical principles and the properties of particles and substances
COLLATED QUESTIONS Electron configuration of atoms and ions of the first 36 elements (using s,p,d notation), periodic trends in atomic radius, ionisation energy, and electronegativity, and comparison of
More informationAtomic chains of groupiv elements and IIIV and IIVI binary compounds studied by a firstprinciples pseudopotential method
Atomic chains of groupiv elements and IIIV and IIVI binary compounds studied by a firstprinciples pseudopotential method R. T. Senger, S. Tongay, E. Durgun, and S. Ciraci* Department of Physics, Bilkent
More informationChapter 8. Periodic Properties of the Element
Chapter 8 Periodic Properties of the Element Mendeleev (1834 1907) Ordered elements by atomic mass Saw a repeating pattern of properties Periodic law when the elements are arranged in order of increasing
More informationGeometry and electronic structure of Vn(Bz)m complexes
West Chester University Digital Commons @ West Chester University Physics College of Arts & Sciences 682004 Geometry and electronic structure of Vn(Bz)m complexes Anil K. Kandalam West Chester University
More informationNanotechnology and Solar Energy. Solar Electricity Photovoltaics. Fuel from the Sun Photosynthesis Biofuels Split Water Fuel Cells
Nanotechnology and Solar Energy Solar Electricity Photovoltaics Fuel from the Sun Photosynthesis Biofuels Split Water Fuel Cells Solar cell A photon from the Sun generates an electronhole pair in a semiconductor.
More informationPhotoabsorption Spectra of Si n and Si n O (n 5)
Commun. Theor. Phys. (Beijing, China) 51 (2009) pp. 751 755 c Chinese Physical Society and IOP Publishing Ltd Vol. 51, No. 4, April 15, 2009 Photoabsorption Spectra of Si n and Si n O (n 5) AN FangFang,
More informationThis manuscript was submitted first in a reputed journal on Apri1 16 th Stanene: Atomically Thick Freestanding Layer of 2D Hexagonal Tin
This manuscript was submitted first in a reputed journal on Apri1 16 th 2015 Stanene: Atomically Thick Freestanding Layer of 2D Hexagonal Tin Sumit Saxena 1, Raghvendra Pratap Choudhary, and Shobha Shukla
More informationIntroduction of XPS Absolute binding energies of core states Applications to silicene
Core level binding energies in solids from firstprinciples Introduction of XPS Absolute binding energies of core states Applications to silicene arxiv:1607.05544 arxiv:1610.03131 Taisuke Ozaki and ChiCheng
More information2D Materials with Strong Spinorbit Coupling: Topological and Electronic Transport Properties
2D Materials with Strong Spinorbit Coupling: Topological and Electronic Transport Properties Artem Pulkin California Institute of Technology (Caltech), Pasadena, CA 91125, US Institute of Physics, Ecole
More informationMustafa Uludogan 1, Tahir Cagin, William A. Goddard, III Materials and Process Simulation Center, Caltech, Pasadena, CA 91125, U.S.A.
Ab Initio Studies On Phase Behavior of Barium Titanate Mustafa Uludogan 1, Tahir Cagin, William A. Goddard, III Materials and Process Simulation Center, Caltech, Pasadena, CA 91125, U.S.A. 1 Physics Department,
More informationFirstprinciples investigations on the structural, electronic and magnetic properties of Crdoped (ZnTe) 12 clusters
J. At. Mol. Sci. doi: 10.4208/jams.100210.102510a Vol. 2, No. 3, pp. 262272 August 2011 Firstprinciples investigations on the structural, electronic and magnetic properties of Crdoped (ZnTe) 12 clusters
More informationIonic Bonding. Example: Atomic Radius: Na (r = 0.192nm) Cl (r = 0.099nm) Ionic Radius : Na (r = 0.095nm) Cl (r = 0.181nm)
Ionic Bonding Ion: an atom or molecule that gains or loses electrons (acquires an electrical charge). Atoms form cations (+charge), when they lose electrons, or anions ( charge), when they gain electrons.
More informationRelaxation dynamics of magic clusters
Relaxation dynamics of magic clusters Y. D. Kim,* M. Niemietz, P. Gerhardt, F. v. GynzRekowski, and G. Ganteför Department of Physics, University of Konstanz, D78457 Konstanz, Germany Using femtosecond
More informationINVESTIGATION OF THE ABSORPTION OF CO 2 IN IONIC LIQUID. Kalyan Dhar 1 * and Syed Fahim 1
Bangladesh J. Sci. Res. 29(1): 4146, 2016 (June) INVESTIGATION OF THE ABSORPTION OF CO 2 IN IONIC LIQUID Kalyan Dhar 1 * and Syed Fahim 1 Dept. di Chimica Materiali e Ingegneria chimica G. Natta, Politecnico
More informationExchange Correlation Functional Investigation of RTTDDFT on a Sodium Chloride. Dimer. Philip Straughn
Exchange Correlation Functional Investigation of RTTDDFT on a Sodium Chloride Dimer Philip Straughn Abstract Charge transfer between Na and Cl ions is an important problem in physical chemistry. However,
More informationSpectroscopic studies ofthe electrical structure oftransition metal and rare earth complex oxides
Available online at www.sciencedirect.com Physica E 21 (24) 712 716 www.elsevier.com/locate/physe Spectroscopic studies ofthe electrical structure oftransition metal and rare earth complex oxides G. Lucovsky
More informationMagnetism in. nanostructured graphene
Magnetism in L. Brey nanostructured graphene Juan José Palacios Funding MEC Spain FIS2004 02356, MAT2007 65487, and CONSOLIDER CSD2007 0010 Generalitat Valenciana Accomp07 054 Dresden, May 29th, 2008 J.
More informationDensity Functional Theory and Genetic Algorithm based studies of Gold clusters and Doped Gold clusters. Masters in Computational Natural Sciences
Density Functional Theory and Genetic Algorithm based studies of Gold clusters and Doped Gold clusters T HESIS SUBMITTED IN PARTIAL FULFILLMENT OF THE REQUIREMENTS FOR THE DEGREE OF Masters in Computational
More informationJournal of Theoretical Physics. Founded and Edited by M. Apostol 50 (2000)
Journal of Theoretical Physics Founded and Edited by M. Apostol 5 () ISSN 45448 Metallic Clusters L. C. Cune and M. Apostol Department of Theoretical Physics, Institute of Atomic Physics, MagureleBucharest
More informationTypes of Bonding : Ionic Compounds. Types of Bonding : Ionic Compounds
Types of Bonding : Ionic Compounds Ionic bonding involves the complete TRANSFER of electrons from one atom to another. Usually observed when a metal bonds to a nonmetal.       + + + + + + + + + +
More information